{'fraction_non_alphanumeric': 0.03341983447888904, 'fraction_numerical': 0.025564595314910926, 'mean_word_length': 4.608062930186824, 'pattern_counts': {'":': 0, '<': 1, '<?xml version=': 0, '>': 1, 'https://': 1, 'lorem ipsum': 0, 'www.': 16, 'xml': 0}, 'pii_count': 0, 'substrings_counts': 0, 'word_list_counts': {'cursed_substrings.json': 0, 'profanity_word_list.json': 0, 'sexual_word_list.json': 0, 'zh_pornsignals.json': 0}}
A novel, rapid, seedless, in situ synthesis method of shape and size controllable gold nanoparticles using phosphates

We hereby report a novel synthesis method of size and shape controllable gold nanoparticles that is rapid, in situ and seedless. Unlike most currently employed size and shape controllable synthesis methods, it takes place in a single step under room temperature within ~15 minutes. While mixtures of gold nanospheres around 70 nm and gold nanoplates with width ranging from 100 nm to 1000 nm can be synthesized in about 15 minutes by standard synthesis method using N-2-hydroxyethylpiperazine-N-2-ethanesulphonic acid (HEPES) to reduce Au(III), gold nanoflowers or mixtures of smaller gold nanospheres and nanoplates can be synthesized with the addition of disodium phosphate (Na2HPO4) or monosodium phosphate (NaH2PO4), respectively. Increasing the concentration of phosphate added significantly reduces the formation time of gold nanoparticles to seconds. By increasing the molar ratio of Na2HPO4: HEPES and NaH2PO4: HEPES, the size of gold nanoflowers and gold nanoparticle mixtures can be tuned from ~60 nm down to 1 nm and from ~70 nm to ~2.5 nm, respectively. The systematic structural changes are accompanied by similarly systematic colour changes associated with shifting of the surface plasmon resonance. The proposed mechanism of the synthesis process is also presented.


Results and Discussions
Estimated GNP formation time. The HEPES reduced GNP synthesis method has been applied and studied for a decade, and it has been reported that the difference of the molar ratio of chloroauric acid and HEPES strongly affects the GNP synthesized 38 . In this study, a molar ratio of 1:10, chloroauric acid to HEPES, has been applied to all syntheses, with or without phosphate added.
During the synthetic progress of all colloidal gold samples, the colour of the system changed from pale yellow, which is the colour of chloroauric acid, into colourless, then became pink/purple/blue, representing the formation of GNPs. The colour changes of the colloidal systems were sufficient to be observed by naked eyes, thus the time from the start of the synthesis to the time at which the colour changed into pink/purple/blue, observed by the naked eye, was recorded as the estimated formation time of the GNP. The estimated formation times, shown in Fig. 1, were recorded to demonstrate the dependence of the rate of GNP formation on the concentration of NaH 2 PO 4 ( Fig. 1 top) or Na 2 HPO 4 ( Fig. 1 bottom) added.
While the estimated formation time of Standard GNP was 15 minutes (±30 seconds), with increased concentration of phosphate, shorter formation time was needed. Note, the estimated GNP formation time became less than 2 seconds when the molar ratio of NaH 2 PO 4 to HEPES was higher than 9, as the colour changed instantaneously after the reaction started; and the estimated formation time stabilized at ~40 seconds when the molar ratio of Na 2 HPO 4 to HEPES was higher than 100. As discussed further in a later section, the dynamics of GNP formation, and the differences for the different reaction systems, are complex and of considerable interest, and will be the subject of a more comprehensive future study. optical properties. The optical characteristics and properties of the GNP suspensions, obtained at 1 hour after synthesis started, are depicted using a combination of photographs and UV/VIS/NIR spectra, as shown in Figs 2 and 3. As shown in Figs 2 and 3, the colour and spectrum of the GNPs varied according to phosphate concentration, which has been converted to the molar ratio of phosphate to HEPES for better understanding.
While the colour of Standard GNP appeared pink, the colour of the ones with NaH 2 PO 4 added became purple and pinkish red when the molar ratio of NaH 2 PO 4 : HEPES was in the range 1.5-6; and when the molar ratio was higher than 9, the colour turned to purple within seconds, then turned dark grey rapidly because of aggregation ( Fig. 2(a)). The higher the molar ratio, the deeper the grey colour of colloidal GNPs became.
The corresponding UV/VIS/NIR spectra of the GNPs synthesized with NaH 2 PO 4 also show systematic trends ( Fig. 2(b,c)). Samples with molar ratio smaller than 12 exhibit 2 LSPR peaks, with one lower than 550 nm (first peak) and the other one higher than 700 nm (second peak). As the GNPs aggregate almost instantly when the molar ratio is higher than 9, the changing trend of spectra appeared different for GNPs with molar ratio higher and lower than 9.
When the molar ratio is smaller than 9, the wavelength of both the first and second peak decreases as the molar ratio increases, and the absorbance of GNPs appears strongest when the molar ratio is 6. On the other hand, when the molar ratio is larger than 9, the wavelength and absorbance of first peak increases along with the molar ratio, then tends to be stable with only slight increase, matching the denser colour, which is caused by the stronger aggregation and larger aggregates. The second peak disappears when the molar ratio is higher than 12, also due to aggregation.
In comparison, the GNPs synthesized with Na 2 HPO 4 added appear bright blue when the molar ratio of Na 2 HPO 4 : HEPES is 0.5-6, and slowly changes to purple and pinkish red when the molar ratio is increased to 30, and then changes into light pink when the molar ratio reaches 60. When the molar ratio is 70 and higher, the colour of GNPs turns pink in seconds, then changes into blue and eventually to grey as the aggregation proceeds. The higher the molar ratio, the faster the aggregation proceeds, and the denser the final colour appears, as the aggregates are larger ( Fig. 3(a)).
The UV/VIS/NIR spectra of this set of samples appears rather well behaved ( Fig. 3(b)). A red-shift of the first peak (the peak smaller than 400 nm) is apparent when the molar ratio increases from 0 to 100, while the corresponding absorbance reaches its highest value when the molar ratio is 3, whereupon a blue-shift of the second peak (the one higher than 500 nm) occurs as the molar ratio increases from 0.5 to 60, along with the decrease of corresponding absorbance, matching the colour change from blue to red/pink. Similar to GNPs synthesized with NaH 2 PO 4 added, the absorbance peaks disappear at high molar ratio because of aggregation.
Crystallinity, size and morphological properties. The size and zeta potential of GNPs synthesized with different molar ratios of phosphate to HEPES were measured using a Zetasizer at ~40 minutes after synthesis started, as presented in Table 1. The average size, calculated from the Size-Number distribution, show trends that match the spectral results. This is consistent with the reports by Haiss et al. that the size and concentration of GNPs within the size range of 5-100 nm can be directly determined from UV-VIS spectra according to corrected Mie theory 40 . The size reaches 350-700 nm when the molar ratio of NaH 2 PO 4 : HEPES is higher than 9, and Na 2 HPO 4 : HEPES is larger than 60, which is because of the rapid aggregation. While Standard GNPs have an average size of ~62 nm, small particles ranging between 1.5-6.5 nm are synthesized when NaH 2 PO 4 : HEPES reaches 1.5-6; and ultra-small particles down to 0.5-3.5 nm are synthesized when the molar ratio of Na 2 HPO 4 : HEPES is 1-12. The trended change of absolute values of zeta potentials is caused by the change of pH due to the increase of phosphate concentration. The measurements of zeta potential values were made to monitor the stability of GNP samples, and the fact that no abrupt changes in zeta potential values was observed is an indication of the stability of the nanoparticles in suspension. www.nature.com/scientificreports www.nature.com/scientificreports/ To further understand the properties of GNPs synthesized with or without phosphate, representative samples were chosen to be analysed using XRD, SEM and TEM.  www.nature.com/scientificreports www.nature.com/scientificreports/ The XRD pattern for GNPs synthesised by all 3 methods are presented in Fig. S1. Standard GNP and GNP synthesized with disodium phosphate added (molar ratio Na 2 HPO 4 : HEPES = 3) exhibited the same characteristic Au crystalline pattern of peaks at 2θ = ~38.5°, ~45.2°, ~65.2°, and ~77.94°, which correspond to Au (111), (200), (220) and (311) Bragg reflections, indicating the formation of GNPs with a face-centred-cubic (fcc) lattice structure (lattice constant = 0.407 nm) [41][42][43] . The XRD pattern for GNP synthesized with monosodium phosphate added (molar ratio NaH 2 PO 4 : HEPES = 3) is slightly different to that of the samples of the other two methods. Although the characteristic Au (111), (200), (220) and (311) peaks are discernible, stronger peaks appear at 2θ = ~32.04°, ~56.74°, and ~66.44°. It has been reported that, while most GNPs crystallize in a fcc lattice structure, tetragonal phase and orthorhombic phases can also be produced 44,45 . Su et al. have discussed the importance of different crystal planes on the surface of polyhedral GNPs 46 , and GNP synthesized by biomass of Aspergillus terreus have been shown to exhibit XRD pattern non characteristic of fcc Au 47 . The peaks of the GNP sample synthesized with monosodium phosphate added can be assigned to Au (110), (211), and (220) Bragg reflections of a strained fcc (lattice constant = 0.397 nm) or tetragonal crystal structure of the surface, with a fcc core. Further study will be carried out to further investigate the differences in gold crystalline structure due to the different synthesis methods.
The SEM and TEM images along with corresponding Size-Number distribution are shown in Fig. 4. The GNPs synthesized using the standard method and with NaH 2 PO 4 added are mixtures of nanospheres and nanoplates, which matches and explains the 2 peaks of the corresponding spectral results. With the presence of nanoplates, a longitudinal surface plasmon resonance at higher wavelength and a transverse surface plasmon resonance at lower wavelength are both created 22,[48][49][50][51] . Thus, for Standard GNP and GNPs synthesized with NaH 2 PO 4 added, the first peak is attributed to the spherical GNPs, while the second peak is attributed to the gold nanoplates. When the molar ratio of NaH 2 PO 4 : HEPES is smaller than 9, a blue-shift of the first peak appears because the diameter of the spherical GNPs decreased ( Fig. 1(c), Table 1) 40,52 . The significant blue-shift of the second peak, which decreased from greater than 1000 nm to ~700 nm, is caused by the size decrease of the nanoplates. As shown in Fig. 4(a,b), the size of the nanoplates of Standard GNP ranges from ~100 nm to ~1000 nm, while the nanoplate size is smaller than 100 nm when the molar ratio of NaH 2 PO 4 : HEPES was 3. When the molar ratio of NaH 2 PO 4 : HEPES was higher than 9, significant aggregation occurred rapidly, whereby gold nanospheres and nanoplates accumulated into large aggregates, and thus, the second peak disappears.
On the other hand, the GNPs synthesized with Na 2 HPO 4 added appear to be gold nanoflowers grown from spherical cores into flowers with petals attached (Fig. 4(c-g)). According to Table 1, the size of GNPs decreases down to less than 1 nm as the molar ratio of Na 2 HPO 4 : HEPES increases from 0.5 to 12. When the molar ratio is 15-40, the size remains between 15 nm to 20 nm. Then when the molar ratio is larger than 50, aggregation occurs rapidly, resulting in large aggregates. In addition to the size change, the number of petals on each nanoflower also decreases as the molar ratio of Na 2 HPO 4 : HEPES increases, which can be seen by comparing the central images of Fig. 4(c-g). While the gold nanoflowers are entirely covered with petals when the molar ratio is less than 3, the petals do not cover the whole surface of the cores when the molar ratio is higher than 3, leading to non-spherical shapes. As the molar ratio increases to greater than 15, only a few petals can be found on each core. The change of GNP shape and size explains the change of the second peak of the corresponding spectral results shown in Fig. 3: when the molar ratio increases from 0.5 to 12, the size decrease of the nanoflowers leads to the blue-shift of the second peak; and when the molar ratio is between 15-40, the LSPR peak wavelength undergoes no further change since the GNP size does not change much. Similarly, stronger aggregation occurs when the molar ratio is further increased, causing large aggregates to sink, leading to the disappearance of the second peak and the decrease of absorbance.
Formation processes of GNP samples. To further understand the synthesis process and mechanism of the GNP samples synthesized with or without phosphates added, representative samples were selected to be monitored using spectroscopy and dynamic light scattering for 48 hours after synthesis started, and SEM/TEM images were also taken within this period.
Synthesis processes of GNPs with/without NaH 2 po 4 added. The Standard GNP samples are formed as a mixture of nanospheres and nanoplates. From Fig. 5(a,b), it can be found that the amount of same sized GNPs increases for ~40 minutes as the synthesis proceeds, since the GNP size stayed relatively stable and the spectral absorbance increased. After that, the GNPs kept stable until ~100 minutes after synthesis started, whereupon the GNPs started to aggregate, and the spectral absorbance decreased. The nanospheres and nanoplates appeared in small clusters before aggregation (Fig. 5(c) left), and assembled into large aggregates after aggregation (Fig. 5(d)  left). For the first ~100 minutes of synthesis, the wavelength positioning of the longitudinal surface plasmon resonance peak created by the nanoplates was larger than 1000 nm, resulting in the rise of absorbance at 700-1000 nm. After ~100 minutes, the nanospheres started to assemble with nanoplates as aggregation started, decreasing the number of nanoplates, which led to the decrease of absorbance at 700-1000 nm.
For GNPs synthesized with NaH 2 PO 4 added, the sample synthesized with the molar ratio of NaH 2 PO 4 : HEPES = 6 was selected as representative, and is referred to as Na6 GNP in the following sections. Similar to Standard GNP, the Na6 GNP was initially synthesized as a mixture of nanospheres and nanoplates, although the average particle size is significantly lower, which may support the proposal that the XRD pattern of Fig. S1 is dominated by the polyhedral surface rather than the Au fcc core. In the first ~20 minutes of synthesis, the number of same sized GNPs increased, and remained relatively stable for the following ~100 minutes. After ~120 minutes of synthesis, the aggregation started as the particle size gradually increased, while the second peak started to red-shift. This could be caused by the aggregation of nanoplates. It has been reported that the increase of the width of nanoplates would lead to a red-shift of the corresponding in-plane dipole plasmon absorption band 22,53-55 , so the red-shift in Fig. 5(b) (right) could be explained by the increase of nanoplate width, because of the aggregation.
www.nature.com/scientificreports www.nature.com/scientificreports/ As the aggregation proceeds to ~400 minutes, the nanospheres and nanoplates assemble (Fig. 5(c) right) into large aggregates, as shown in Fig. 5(d) right, causing large particle sizes (Fig. 5(a) right) and the decrease of overall spectral absorbance (Fig. 5(b) right). (c-g) GNPs synthesized with Na 2 HPO 4 added, at molar ratios of Na 2 HPO 4 : HEPES = 0.5, 1.5, 3, 12, 30, respectively. SEM/TEM images were taken between 1-2 hours since synthesis started, and the size-number distribution histogram was measured at ~40 minutes since synthesis started. www.nature.com/scientificreports www.nature.com/scientificreports/ Overall, the synthesis processes of Standard GNP and GNP synthesized with NaH 2 PO 4 added were similar: a mixture of gold nanospheres and nanoplates was synthesized, then aggregation began at different time points depending on the concentration of NaH 2 PO 4 added. As shown in Fig. 1(b) top, the higher concentration of NaH 2 PO 4 added, the faster the aggregation would happen. www.nature.com/scientificreports www.nature.com/scientificreports/ Synthesis processes of gold nanoflowers with Na 2 Hpo 4 added. The GNPs synthesized with Na 2 HPO 4 added were gold nanoflowers, as shown in Fig. 4. The samples synthesized with molar ratio of Na 2 HPO 4 : HEPES = 3, 12 and 30 were selected as representative, and will be referred to as Na 2 3, Na 2 12 and Na 2 30 GNP, respectively in the following sections. Similarly, the GNPs synthesized with Na 2 HPO 4 added reached stable particle sizes within the first few minutes, whereupon the amount of particles increased until the synthesis process finished, leading to the increase of the spectral absorbance ( Fig. 6(a,b)). The time of these synthesis processes www.nature.com/scientificreports www.nature.com/scientificreports/ varied with different concentrations of Na 2 HPO 4 added. The higher concentration of Na 2 HPO 4 added, the shorter the time needed for the synthesis process to come to completion ( Fig. 1(b) bottom).
The spectra of these 3 samples appears rather interesting. While the second peaks of each sample, which are caused by the localized surface plasmon resonance of gold nanoflowers, stayed rather stable over time once synthesis was complete, the first peaks changed with the same trend. The first peak of Na 2 3 GNP appeared at 310 nm, after ~17 minutes of synthesis, then red-shifted to 335 nm while the absorbance increased at the same time until ~1 hour after synthesis started; then the red-shift continued rather slowly to 340 nm over the time, with absorbance decreasing slightly. Similarly, the first peaks of Na 2 12 and Na 2 30 GNP both appeared at 330 nm after ~10 minutes, then red-shifted to 340 nm with increased absorbance within 10 minutes. The peak of Na 2 12 GNP www.nature.com/scientificreports www.nature.com/scientificreports/ did not change until ~7 hours after synthesis, when the absorbance started to increase significantly. Similarly, the peak of Na 2 30 GNP stayed unchanged until ~2 hours after synthesis started, whence the absorbance increased abruptly; then the absorbance decreased slightly after ~24.5 hours of synthesis. On the other hand, the second peaks of Na 2 3, Na 2 12 and Na 2 30 GNP remained stable until ~11.5 hours, ~7 hours and ~5 hours after synthesis started, respectively, whence the absorbance started to decrease slightly because of the aggregation. Higher concentration of NaH 2 PO 4 added caused faster aggregation of GNP samples as well.
From Fig. 6(c), it can be seen that the nanoflowers are grown from spherical cores into flowers, with smaller particles in the images demonstrating the uncomplete growth. Relating the UV/VIS/NIR spectral results of these gold nanoflowers as shown in Fig. 3, it should be noticed that, in contrast to common nanoflowers which have 2 LSPR peaks, located at 520-600 nm, and the other one, caused by aggregation, located at longer wavelength [56][57][58][59] , these nanoflowers synthesized with Na 2 HPO 4 added only exhibit one LSPR band in the VIS/NIR region. This phenomenon, as previously reported by Hong Yuan et al. and Wei Wang et al., could be caused by the difference in synthesis mechanisms: instead of the aggregation between grown petals and cores, these nanoflowers were formed by a second growth on cores 60,61 . The cores grew from very small into relatively larger spherical particles, then a second growth started, resulting in the petals on the cores. The HRTEM and corresponding FFT images in Fig. 6(c) showed that the petals selectively grew in the <111> direction, and had same d-spacing with cores of 0.221 nm. The presence of larger flowers and smaller cores could also explain the 2 different average sizes of Na 2 12 and Na 2 30 GNP measured by Zetasizer in Fig. 6(a).
proposed formation scheme. As the different major facets of crystalline gold have similar chemistry and surface free energies, an exact mechanism of the shape control of GNPs has proven nontrivial to formulate 29 . We hereby propose possible formation schemes of GNPs with or without phosphates added during the synthesis processes, as shown in Fig. 7.
For a standard HEPES reduced synthesis of GNPs, the reaction process has been well documented 39,62 : HEPES reduces Au(III), creating Au(II) and cationic free radicals of HEPES; then the disproportionation of Au(II) creates Au(III) and Au(I); and Au(I) continues to react with HEPES, creating Au(0) and more cationic HEPES free radicals. The Au(0) assembles into very small gold nanoparticle cores first. Then, during the growth process, the HEPES free radicals attach to the surface of the particles, stabilizing them from aggregation and controlling the particle size, as they create a fixed volume of space in which the GNP can grow 63,64 . The proposed structures of gold nanospheres and nanoplates are shown in Fig. 7(a).
With the addition of NaH 2 PO 4 , phosphate ions are introduced to the reaction system. The phosphate ions form hydrogen bonds with the HEPES free radicals, as shown in Fig. 7(b) (nanosphere), creating effectively longer polymer chains attached to the particle surfaces. With larger attachments, the space for nanospheres to grow is decreased, leading to smaller size particles. Similarly, with the ability of forming more than one hydrogen bond, the phosphate ions can also link several HEPES free radicals, as shown in Fig. 7(b) (nanoplate). With large polymer chains attached, the width and thickness is restricted to a much smaller range, compared to the conditions for growth of Standard GNP. When the molar ratio of NaH 2 PO 4 : HEPES is lower than 9, the more NaH 2 PO 4 added, the more phosphate ions are brought into the system, creating more hydrogen bonds and thus larger polymer clusters attached to GNPs. Thus, a higher molar ratio of NaH 2 PO 4 : HEPES leads to smaller particle sizes. When the molar ratio of NaH 2 PO 4 : HEPES is further increased, the overloading of ions in the system destroys the synthesis environment and leads to rapid formation and aggregation. A similar trend has been reported for the ascorbic acid reduced, CTAB stabilized, GNP synthesis system, whereby the addition of small concentrations of iodide ions changes the morphology of GNPs synthesized, from nanorods (mixed with nanospheres) into nanoplates (mixed with nanospheres), and the higher the concentration of iodide ions added, the smaller the size of GNPs synthesized 21 .
It has been reported that the pH value plays a very important role in the synthesis of GNPs, as it can change the shape and size of GNPs synthesized 39,65,66 . It has also been reported that, using the same synthesis method, nanorods or mixtures of gold nanospheres and nanoplates were synthesized when the pH was smaller than 7, and gold nanoflowers were synthesized when the pH was equal to and larger than 7 67,68 .
In our study, with the addition of Na 2 HPO 4 , the pH value of the system increased to larger than 7, creating an alkaline environment, which inhibited the formation of cationic HEPES free radicals. Thus, insufficient stabilizer ions were present in the system for the formation of nanoplates. Under these conditions, the phosphate ions create hydrogen bonds with HEPES free radicals, and large polymer clusters attach to the particle surface, restricting the growth of gold cores, as shown in Fig. 7(c). Under an alkaline environment, a second growth of petals happens on the cores, resulting in the nanoflowers. With the increase of phosphate ion amount, the size of attached polymer clusters increases, leaving less space for petals to grow, which explains the decrease of petal amount as the molar ratio of Na 2 HPO 4 : HEPES increases.
The first peak of these nanoflowers could be caused by the coordinating action between HEPES free radicals and gold under alkaline conditions. As previously reported, the absorption peak at 346 nm has been noticed for GNPs synthesized using HEPES and 2-morpholinoethanesul-fonic acid (MES), and was proposed to be caused by the formation of nitro-compounds 39 . The red-shift of this peak could be caused by the amount decrease of HEPES free radicals coordinated with gold, and the change in absorption was caused by the amount change of complexes. Additional analysis and further research on the mechanisms of GNP formation according to this method will be carried out to support the proposed scheme.

Conclusion
In summary, we have developed a novel bottom-up in situ synthesis method of shape and size controllable GNPs. The method is rapid, taking less than 15 minutes, and doesn't need any seed. The GNPs are HEPES reduced with phosphate concerted. With NaH 2 PO 4 added, mixtures of gold nanospheres and nanoplates sizing from ~70 nm to ~2.5 nm could be synthesized by increasing the molar ratio of NaH 2 PO 4 : HEPES from 0 to 6. And by adding (2019) 9:7421 | https://doi.org/10.1038/s41598-019-43921-0 www.nature.com/scientificreports www.nature.com/scientificreports/ Na 2 HPO 4 into the synthesis system, gold nanoflowers sizing from ~60 nm down to ultra-small as less than 1 nm could be synthesized, with the amount of petals decreases as the molar ratio of Na 2 HPO 4 : HEPES increases. The GNP formation time decreases as the concentration of phosphate added increases. The LSPR peaks of the gold nanoflowers could be tuned from 605 nm to 540 nm. With such small size and controllable morphology, this synthesis method holds great potential in the application of surface enhanced Raman scattering imaging for cells, biolabling, plasmonic waveguiding and so on.
Synthesis of colloidal GNPs. A 1 mM stock solution of chloroauric acid and 10 mM stock solution of HEPES buffer was made by dissolving hydrogen tetrachloroaurate in water and diluting purchased HEPES buffer with water accordingly. Different concentrations of phosphate stock solutions were similarly prepared by dissolving NaH 2 PO 4 and Na 2 HPO 4 in water.
In a standard synthesis process of GNPs, 200 µL of 1 mM chloroauric acid were mixed with 200 µL of 10 mM HEPES buffer and 600 µL of water under room temperature. The colour changed from pale yellow to colourless, then gradually changed to pink within ~15 minutes, indicating the formation of GNPs. The GNPs synthesized by this method are referred to as Standard GNP in the following sections.
On the basis of standard process, in the synthesis processes with phosphate added, similar procedures were followed, except that 200 µL of 1 mM chloroauric acid were mixed with 200 µL of 10 mM HEPES buffer and 600 µL of phosphate stock solutions with systematically varied concentrations.
Characterization of GNPs. X-Ray Diffraction (XRD) analysis was performed using a Siemens diffractometer with a monochromatic Cu-Kα 1 source operated at 40 keV and 30 mA. Samples were deposited from suspension onto the sample holder and allowed to dry, until a uniform coating was achieved.
Scanning electron microscope (SEM) images of GNPs were recorded by a Hitachi SU6600 FESEM instrument, and transmission electron microscope (TEM) images of GNPs were recorded by a JEOL JEM-2100 Electron Microscope instrument. Samples prepared for SEM imaging were dropped onto silicon wafers and spun for 2.5 minutes to dry in the air for ~1.5 hours after the synthesis reaction started. Samples prepared for TEM imaging were dropped onto copper grid with ultra-thin carbon film to dry in the air for ~1.5 hours after the synthesis reaction started. An accelerating voltage of 20 kV was used for all samples for SEM imaging, and 200 kV was used for all samples for TEM imaging.
A Perkin Elmer Lambda 900 UV/VIS/NIR Spectrometer was used to measure the absorption spectra of the GNPs in the 300-1000 nm region. The absorption spectra were used to monitor the formation of GNPs, and to characterize and discriminate different samples.
A Zetasizer Nano ZS Analyser from Malvern Instruments, Worcestershire, UK was used to measure the hydrodynamic particle sizes and zeta potentials of different GNP samples.
A Thermo Scientific ™ Orion ™ 3-Star Benchtop pH Meter was used to measure pH values of the GNP samples.

Data Availability
All data generated or analysed during this study are included in this published article (and its Supplementary Information files).